1 - Oregon Department of Geology and Mineral Industries
28 Ferruginous bauxite STATE DEPARTMENT OF GEOLOGY AND MINERAL INDUSTRIES • vol.ll no.4 The other raw material, given the name ferruginous bauxite, is of laterite origin, located in sizeable deposits in Northwestern Oregon, espeoially Columbia County.ll Although the oompositions vary with location, two different samples used by these investigators show the following analyses, the first material (with the lower silioa ccntent) is of the olassification known as "upper pisolitio fine," while the seoond is a typical mining mix." H 2 0 3 Fe 203 Ti02 51°2 Ignition loss ill pct 34.20 33.?? 6.43 6.62 18.71 ill pet 34.20 34.00 6.40 ? 50 l5.?O Both of these samples were obtained from Alcoa Mining Company which is conducting experiments as to the uses of this material as an aluminum source. The samples of this bauxite are located on the ternary diagram, on an iron- and titanium-free basis. The eoonomic study of these deposits has not been so thoroughly investigated by the authors as the kaolin clays, but it seems probable that the bauxite deposits would provide a satisfactory source from the standpoint of cost of mining, available supply, eto. 12 The deposits average about fifteen feet in depth, with an overburden of It to 30 feet, with the former figure the more common, mostly of silt. l ; Experimental Work Castle-Rook clay The first experiments were performed with Castle-Rock clay tc which technical grade lime was added tc make up the oalcium cxide content of the cement, while technical grade of alumina was used to bring the composition down nearer to the desired area of oements. Fusion was first attempted in a small induotion furnace. But this furnaoe failed to get up to the necessary heat for complete fUSion. The authors then used a single-phase arc furnace for which they built a speoial graphite crucible in order to fuse small-run batches of cement.* The results of the runs on the clay as well as those obtained later on the bauxite are tabUlated in Table 2. After a number of unsuccessful runs, it was decided that experimentation further with the clay as a raw material would be useless, because of the amount of pure alumina that had to be added. For instanoe, the makeup of Run no. 6 was: clay - 370 grams, pure alumina - 550 grams, and lime - 645 grams. It can be seen that very little use was made of the clay, and the alumina would naturally be too costly as a raw material. In addition, it is to be remembered that the silica and alumina are tied together in the elay in a moleoular struoture and it is very probable that moro rigorous eonditions would be required to break these bonds and make the cement molecules. llKelly, J. Vo, 'High alumina-iron laterite depcsits, Columbia County, Oregon": U.S. Bur. Uines Rept. Inv. 4081, 1947. 12Libbey, F. W., Lowry, W. D., and Mason, R. S., "Ferruginous bauxite deposits in northwestern Oregon": Eoonomio Geology, vol. 41, no.3, pp. 246-265, 1?46. 13Kelly, J. v., OPe oit. * The original theSis fully desoribes the perfDraanee of the furnace and the behavior of the clay during experimentation.